This item was submitted to Loughborough University as a PhD thesis by the author and is made available in the Institutional Repository
(https://dspace.lboro.ac.uk/) under the following Creative Commons Licence conditions.
For the full text of this licence, please go to: http://creativecommons.org/licenses/by-nc-nd/2.5/
Further Process Understanding and
Prediction on Selective Laser Melting
of Stainless Steel 316L
A Doctoral Thesis Submitted in Partial Fulfilment of the
Requirements for the Award of Doctor of Philosophy of
Wolfson School of Mechanical and Manufacturing Engineering
Additive Manufacturing (AM) is a group of manufacturing technologies which are capable to produce 3D solid parts by adding successive layers of material. Parts are fabricated in an additive manner, layer by layer; and the geometric data can be taken from a CAD model directly. The main revolutionary aspect of AM is the ability of quickly producing complex geometries without the need of tooling, allowing for greater design freedom. As one of AM methods, Selective Laser Melting (SLM) is a process for producing metal parts with minimal subtractive post-processing required. It relies on the generation and distribution of laser generated heat to raise the temperature of a region of a powder bed to above the melting point. Due to high energy input to enable full melting of the powder bed materials, SLM is able to build fully dense metal parts without post heat treatment and other processing.
Successful fabrications of parts by SLM require a comprehensive understanding of the main process controlling parameters such as energy input, powder bed properties and build conditions, as well as the microstructure formation procedure as it can strongly affect the final mechanical properties. It is valuable to control the parts’ microstructure through controlling the process parameters to obtain acceptable mechanical properties for end-users. In the SLM process, microstructure characterisation strongly depends on the thermal history of the process. The temperature distribution in the building area can significantly influence the melting pool behaviour, solidification process and thermal mechanical properties of the parts. Therefore, it is important to have an accurate prediction of the temperature distribution history during the process.
The aim of this research is to gain a better understanding of process control parameters in SLM process, and to develop a modelling methodology for the
prediction of microstructure forming procedure. The research is comprised of an experiment and a finite element modelling part.
Experimentation was carried out to understand the effect of each processing control parameters on the final part quality, and characterise the model inputs. Laser energy input, build conditions and powder bed properties were investigated. Samples were built and tested to gain the knowledge of the relationship between samples’ density and mechanical properties and each process control factor. Heat transfer model inputs characterisation, such as defining and measuring the material properties, input loads and boundary conditions were also carried out via experiment.
For the predictive modelling of microstructure, a methodology for predicting the temperature distribution history and temperature gradient history during the SLM process has been developed. Moving heat source and states variable material properties were studied and applied to the heat transfer model for reliable prediction. Multi-layers model were established to simulate the layer by layer process principles. Microstructure was predicted by simulated melting pool behaviour and the history of three dimensional temperature distribution and temperature gradient distribution. They were validated by relevant experiment examination and measurement.
I am deeply indebted to my supervisors Prof. Richard Hague, Dr. Christopher Tuck, Prof. Ian Ashcroft and Prof. Ricky Wildman for their guidance, kindness, suggestions, patience and supervision throughout the entire research. This work would not have been possible without their insight and awareness. Special thanks to Dr. Christopher Tuck for his suggestions on my thesis writing. His encouragement and understanding helped me sail through the hard times.
Sincere thanks to technician Andy Sandaver and Mark East for their guidance and help during the experimentation of this research, as well as being my best friends and supporting me all the time. Special thanks to IT technician Darren Smith who saved my research data from a broken hard drive. Thanks are also due to Dr. Yau Yau Tse for her help on metal phase characterisation experiment and Dr. Sozon Tsopanos for his help in the initial stage of the research.
I am grateful to all the staff of the Wolfson School of Mechanical and Manufacturing Engineering, Loughborough University for their support and help, especially Andy Price, Clive Turner, Alan Trahar, Jagpal Smith, Dave Britton, Chris Harris, Bob Temple, Keven Smith and Richard Price. Thanks to all the members of the Additive Manufacturing Research Group (AMRG). I am sincerely grateful to Mark Hardy, Dr. Candi Majewski, Dr. Helen Thomas and Jiaming Bai for all their help, encouragement, kindness and friendship.
Finally, I would like to thank Dr. Chris Sutcliffe and Dr. Yau Yau Tse for their efforts as external and internal examiners respectively.
ContentsAbstract ... i Acknowledgement ... iii Contents ... iv List of Figures ... x List of Tables... xv
List of Symbols ... xvii
List of Acronyms ... xix
1 Introduction ... 1 1.1 Background ... 1 1.2 Scope of Research ... 3 1.3 Research Methodology ... 4 1.4 Research Novelty ... 5 1.5 Thesis Structure ... 5 2 Literature Review ... 8 2.1 Additive Manufacturing ... 8 2.1.1 Classification ... 9 2.1.2 Liquid-based processes ... 10 2.1.3 Solid-based processes ... 10 2.1.4 Powder-based processes ... 11
2.2 Direct Metal Laser Fabrication ... 13
2.2.1 Laser scanning systems ... 13
2.2.2 Laser-Material interactions ... 17
2.3 Selective Laser Melting ... 19
2.3.1 Process control factors ... 20
2.3.2 Optical scanning system ... 22
2.3.3 Process scanning strategy ... 23
2.3.4 Process environment ... 25
2.3.5 Raw material used in SLM process ... 26
2.3.6 Powder flowability ... 28
2.3.7 Effect of chemical elements ... 29
2.3.8 Laser energy absorption ... 29
2.3.9 Microstructural development ... 30
2.4 Heat transfer in the powder bed ... 34
2.4.1 Thermal conductivity ... 34
2.4.2 Melting energy ... 35
2.4.3 Residual stresses ... 36
2.4.4 Thermal shrinkage ... 37
2.5 Heat Transfer Modelling in Selective Laser Melting ... 37
2.5.1 Heat transfer theory on general laser processing work ... 38
2.5.2 Previous solutions of laser processing simulations... 39
2.5.3 Input heat source development for laser processing work ... 41
2.5.4 Powder bed studies for the thermal properties ... 44
2.5.5 Previous modelling works for the SLM process ... 46
2.6 Summary ... 47
3 Experimental Research Methods ... 49
3.1 Introduction ... 49
3.2 Selective laser melting equipment ... 50
3.2.2 Building chamber ... 52
3.2.3 Machine operating software ... 53
3.2.4 Process control parameters file ... 54
3.3 SLM Process Understanding and Optimisation ... 57
3.3.1 Optical scanning system examination ... 57
3.3.2 Process scanning strategy study ... 60
3.3.3 Building conditions investigation ... 63
3.4 Raw material characterisation ... 64
3.4.1 Material used in the study ... 64
3.4.2 Storage and preparation ... 65
3.4.3 Particle shape, size distribution and powder bed density ... 67
3.4.4 Powder flowability measurement ... 69
3.4.5 Effect of particle size distribution on parts quality ... 70
3.4.6 Powder sustainability study ... 70
3.5 Model inputs characterisation ... 72
3.5.1 Powder bed density ... 73
3.5.2 Thermal conductivity ... 73
3.5.3 Specific heat capacity ... 74
3.6 Microstructure examination ... 76
3.7 Summary ... 76
4 Finite Element Modelling Methods ... 78
4.1 Introduction ... 78
4.2 Geometry and boundary conditions ... 80
4.3 Meshing methodology and choice of elements ... 84
4.3.1 Two dimensional Tri 3 ... 86
4.3.3 Two dimensional Quad 4 ... 88
4.3.4 Two dimensional Quad 8 ... 89
4.3.5 Element type and results accuracy ... 90
4.4 Moving heat source application ... 92
4.5 States variable material properties study ... 94
4.6 Multi-layers model establishment ... 95
4.7 Summary ... 97
5 Results & Discussions - SLM Process Control Parameters ... 98
5.1 Introduction ... 98
5.2 Energy input study ... 99
5.2.1 Laser profiles examination ... 99
5.2.2 Laser focus position and energy intensity study ... 101
5.2.3 Building area variation ... 106
5.2.4 Scanning speed ... 109 5.2.5 Hatch distance ... 112 5.2.6 Re-melting process ... 116 5.2.7 Building direction ... 117 5.3 Building conditions ... 122 5.3.1 Processing environment ... 122
5.3.2 Effect of gas flow ... 126
5.3.3 Pre-heating study ... 129
5.4 Summary ... 130
6 Results & Discussions - Raw Material Characterisation ... 132
6.1 Introduction ... 132
6.2 Particle shape and size distribution ... 132
6.4 The effect of particle size distribution... 135
6.4.1 Density of the finishing parts ... 137
6.4.2 Surface roughness of the finishing parts ... 138
6.4.3 Tensile strength and elongation of the finishing parts... 140
6.4.4 Hardness of the finishing parts ... 142
6.5 Powder sustainability study ... 144
6.5.1 LPW powder monitoring ... 144
6.5.2 SO powder monitoring ... 150
6.6 Summary ... 154
7 Results & Discussions - Model Inputs Characterisation ... 156
7.1 Introduction ... 156
7.2 Material Properties... 156
7.2.1 Density ... 157
7.2.2 Thermal conductivity ... 157
7.2.3 Specific heat capacity ... 159
7.3 Loads ... 162
7.4 Boundary Conditions ... 162
7.4.1 Top surface ... 162
7.4.2 Bottom surface ... 163
7.5 Summary ... 165
8 Results & Discussions - Heat transfer Model Establishment ... 166
8.1 Introduction ... 166
8.2 Moving heat source application ... 167
8.2.1 Melt pool formation ... 167
8.2.2 Laser processing parameters effect ... 168
8.4 Multi-layers model establishment ... 173
8.5 Summary ... 185
9 Results & Discussions - Microstructure Prediction and Validation ... 187
9.1 Introduction ... 187 9.2 Microstructure prediction ... 187 9.3 Microstructure examination ... 189 9.3.1 Horizontal view ... 189 9.3.2 Vertical view ... 193 9.3.3 Phase identification ... 195 10 Discussions ... 198 10.1 Introduction ... 198
10.2 Connection between the works ... 198
10.3 Energy input and building conditions ... 200
10.4 Powder material’s properties effect ... 201
10.5 Temperature distribution history and microstructure prediction and validation ... 202
10.6 Linkage and contribution to SLM research area ... 203
11 Conclusions and Future Works ... 205
11.1 Conclusions ... 205
11.2 Future works ... 206
List of Figures
Figure 1-1 Main thesis structure ... 7
Figure 2-1 Family tree of Additive Manufacturing Technologies  ... 9
Figure 2-2 Gaussian beam mode profiles  ... 14
Figure 2-3 Gaussian beam parameters after focusing  ... 16
Figure 2-4 Schematic of the Selective Laser Melting process ... 20
Figure 2-5 Working principle of F-theta lens  ... 22
Figure 2-6 Schematic of some input process parameters ... 23
Figure 2-7 C-Fe phase diagram  ... 31
Figure 2-8 Fe-Cr phase diagram  ... 32
Figure 2-9 Fe-Ni phase diagram  ... 32
Figure 2-10 Fe-Cr-Ni-C phase diagram  ... 33
Figure 2-11 Heat distribution in the powder bed ... 35
Figure 2-12 Schematic model for Goldak heat source  ... 43
Figure 2-13 Contact radius between two spherical particles with the same radius R ... 45
Figure 2-14 Close-packed structure of particles... 45
Figure 3-1 MCP SLM-Realizer 100 ... 51
Figure 3-2 Optics system inside MCP SLM-Realizer 100 ... 52
Figure 3-3 Process chamber in MCP SLM-Realizer 100 ... 53
Figure 3-4 Operating software in MCP SLM-Realizer 100 ... 54
Figure 3-5 Material file description Part 1, point distance setting for different scans ... 55
Figure 3-6 Material file description part 2, major controllable parameters settings ... 56
Figure 3-7 Material file description part 3, scan strategy control ... 57
Figure 3-8 Laser mark on the laser markable label ... 59
Figure 3-9 Microstructure of part shows melting pool shape in vertical view 62 Figure 3-10 Store package for the powder used in the study ... 66
Figure 3-12 Design of container built for powder bed density measurement 68 Figure 3-13 Powder degradation after one year processing, a) and b) are
showing different particles with same degradation ... 71
Figure 3-14 Sample dimensions for thermal conductivity apparatus ... 73
Figure 4-1 Overall methodology of the heat transfer model ... 79
Figure 4-2 Boundary conditions for each cuboid surface ... 81
Figure 4-3 Process properties during the SLM process ... 83
Figure 4-4 Element types provided by ABAQUS/CAE  ... 85
Figure 4-5 Tri 3 element size study, figure a) to d) are heat flux results, figure e) to h) are temperature results at different mesh sizes ... 86
Figure 4-6 Tri 6 element size study, figure a) to d) are heat flux results, figure e) to h) are temperature results at different mesh sizes ... 87
Figure 4-7 Quad 4 element size study, figure a) to d) are heat flux results, figure e) to h) are temperature results at different mesh sizes ... 88
Figure 4-8 Quad 8 element size study, figure a) to d) are heat flux results, figure e) to h) are temperature results at different mesh sizes ... 89
Figure 4-9 Compare different element type and size for result accuracy examination... 91
Figure 4-10 UMAT structure for states variable material properties ... 95
Figure 4-11 Schematic for establishing multi-layers model ... 96
Figure 5-1 Laser beam profile under 25W power, 14.50mm lens focus position ... 101
Figure 5-2 Laser beam profile under 25W power, 14.00mm lens focus position ... 102
Figure 5-3 Laser beam profile under 25W power, 14.30mm lens focus position ... 102
Figure 5-4 Laser beam profile under 25W power, 14.80mm lens focus position ... 103
Figure 5-5 Firing laser onto laser markable label under different lens position value ... 104
Figure 5-6 Marks on the laser paper under optical microscope, same magnification for all three images ... 104
Figure 5-7 Top view of building area variation study orientation ... 106 Figure 5-8 Tensile test specimens built in parallel with gas flow direction . 109
Figure 5-9 Cross sections of parts built by 4 different scanning speeds .... 111
Figure 5-10 Thin wall built for hatch distance study ... 113
Figure 5-11 Measured densities of thin walls by different scanning speeds ... 113
Figure 5-12 Measured thickness of thin walls by different scanning speeds ... 114
Figure 5-13 Average density on different hatch distance ... 115
Figure 5-14 Top surface improvement through re-melting process, L is the original part, R has been re-melted on the top surface ... 116
Figure 5-15 Tensile test specimens built for build directions study ... 117
Figure 5-16 Cross section of round tensile test specimen built on X direction ... 118
Figure 5-17 Tensile test specimens with/without topping up delay during the process have been pulled ... 120
Figure 5-18 Tensile test specimens with/without topping up delay during the process have been pulled ... 121
Figure 5-19 Chemical composition comparison between fresh, recycled and oxidised stainless steel 316L powder ... 123
Figure 5-20 SEM images of oxidised stainless steel 316L particles ... 124
Figure 5-21 Dark particles generated by improper high laser energy intensity ... 124
Figure 5-22 SEM image of dark particles generated by improper high laser energy intensity ... 125
Figure 5-23 Results from gas flow effect study ... 126
Figure 5-24 Tensile test specimens were built for dark particles effect study ... 128
Figure 5-25 Break specimens built for dark particles effect study ... 129
Figure 6-1 a) Osprey, b) LPW powder under SEM, mag=500x ... 133
Figure 6-2 Particle size distribution measured by Mastersizer 2000 ... 133
Figure 6-3 Cross section of parts built on 300mm/s, a) Osprey, b) LPW ... 137
Figure 6-4 Side surface roughness for both SO and LPW parts ... 139
Figure 6-5 Top surface roughness for both SO and LPW parts ... 139
Figure 6-6 UTS of both SO and LPW parts ... 141
Figure 6-8 Hardness under different scanning speeds ... 142 Figure 6-9 LPW powder in different stages, examined by SEM ... 145 Figure 6-10 Particle size distribution comparisons for LPW powder ... 146 Figure 6-11 Crystalline orientation maps of two particles random selected from LPW virgin powder ... 148 Figure 6-12 Crystalline orientation maps of two particles random selected from LPW powder after 800 hours processing ... 149 Figure 6-13 SO powder in different stages, examined by SEM ... 151 Figure 6-14 Particle size distribution comparison for SO powder ... 152 Figure 7-1 Powder bed thermal conductivity based on different sidewall thickness ... 158 Figure 7-2 Specific heat thermal curve for stainless steel 316L powder .... 160 Figure 7-3 Calculated specific heat capacity of powder bed ... 160 Figure 7-4 Bottom surface temperature of the build substrate monitored during an 8 hour build ... 163 Figure 7-5 Temperature distribution on the build substrate when a constant 45°C temperature applied onto its bottom surface ... 164 Figure 8-1 Melting pool formation from FE modelling ... 167 Figure 8-2 Temperature distribution at different recording time using
200mm/s scanning speed, a at 4s, b at 8s, c at12s, d at 16s ... 168 Figure 8-3 Temperature distribution under 300mm/s (a) and 150mm/s (b) 169 Figure 8-4 Melting pool size and maximum temperature under four different scanning speeds ... 169 Figure 8-5 Moving heat source applied to a solid material state medium .. 171 Figure 8-6 Moving heat source applied to a powder state medium ... 171 Figure 8-7 Moving heat source applied to the states variable medium ... 172 Figure 8-8 Temperature distribution result (top), temperature history for 3 selected nodes (bottom), layer 1 ... 174 Figure 8-9 Temperature distribution result (top), temperature history for 3 selected nodes (bottom), layer 2 ... 175 Figure 8-10 Temperature distribution result (top), temperature history for 3 selected nodes (bottom), layer 3 ... 176 Figure 8-11 Temperature distribution result (top), temperature history for 3 selected nodes (bottom), layer 4 ... 177
Figure 8-12 Temperature distribution result (top), temperature history for 3 selected nodes (bottom), layer 5 ... 178 Figure 8-13 Temperature distribution result (top), temperature history for 3 selected nodes (bottom), layer 6 ... 179 Figure 8-14 Temperature distribution result (top), temperature history for 3 selected nodes (bottom), layer 7 ... 180 Figure 8-15 Temperature distribution result (top), temperature history for 3 selected nodes (bottom), layer 8 ... 181 Figure 8-16 Temperature distribution result (top), temperature history for 3 selected nodes (bottom), layer 9 ... 182 Figure 8-17 Selected nodes’ peak temperatures in each layer ... 183 Figure 8-18 Temperature history for the middle node from layer 1 to layer 9 ... 185 Figure 9-1 Isothermal transformation diagram for carbon steel  ... 188 Figure 9-2 SLM stainless steel microstructure under SEM, mag=500,
horizontal view ... 190 Figure 9-3 SLM stainless steel microstructure under SEM, mag=1000,
horizontal view ... 190 Figure 9-4 Temperature history of five nodes picked from the centre to the edge of the heat affected zone... 191 Figure 9-5 Nano indentations on polished SLM thin wall horizontal side ... 192 Figure 9-6 Nano indentations on the central area and surrounded grains . 193 Figure 9-7 SLM stainless steel microstructure under SEM, mag=500, vertical view ... 194 Figure 9-8 SLM stainless steel microstructure under SEM, mag=1000,
vertical view ... 194 Figure 9-9 Crystalline orientation maps of SLM thin wall part, horizontal view ... 196 Figure 9-10 Crystalline orientation maps of SLM thin wall part, vertical view ... 197
List of Tables
Table 2-1 Absorption of powder materials at different wavelength  ... 18
Table 2-2 Main SLM process control factors ... 21
Table 2-3 Input process parameters of SLM ... 24
Table 3-1 Chemical composition provided by suppliers (unit: wt%) ... 65
Table 5-1 Laser power detected under static mode ... 99
Table 5-2 Laser power detected under scanning mode ... 99
Table 5-3 Average density of samples built under different lens positions . 105 Table 5-4 Measured gauge area diameter of specimens ... 107
Table 5-5 Measured density of specimens ... 107
Table 5-6 Tensile strength (UTS) of specimens ... 108
Table 5-7 Average densities of parts built by 4 different scanning speeds 111 Table 5-8 Tensile strength and elongation at break of parts built by 4 scanning speeds ... 112
Table 5-9 Tensile strength and elongation at break under different build directions ... 119
Table 5-10 Tensile strength and elongation at break with/without topping up delay, samples were built in Z direction ... 120
Table 5-11 Tensile strength and elongation at break with/without topping up delay, samples were built in X direction ... 122
Table 5-12 Chemical composition of one oxidised stainless steel 316L particle ... 123
Table 5-13 Average tensile strength of specimens built for dark particles effect study... 128
Table 5-14 Average density, tensile strength and elongation for pre-heating study ... 130
Table 6-1 Measured apparent density, powder bed density and tapped density ... 134
Table 6-3 Specimens built parameters using different scanning speeds for particle size distribution effect study ... 136 Table 6-4 Specimens built parameters using different laser beam diameters for particle size distribution effect study ... 136 Table 6-5 Average density of parts built using different scanning speeds . 137 Table 6-6 Average density of parts built using different laser beam diameters ... 138 Table 6-7 Average mechanical properties comparison for LPW parts ... 147 Table 6-8 Average mechanical properties comparison for SO parts ... 154
List of Symbols
r radial distance from the centre axis of the beam
z axial distance from the beam's narrowest point (the "waist")
I0 intensity at the centre of the beam at its waist
w(z) radius at which the field amplitude and intensity drop to 1/e and
1/e2 of their axial values respectively
w0 waist size
η characteristic impedance of the medium in which the beam is
zR distance along the propagation direction of the laser beam from the waist to the place where the area of the cross section is
doubled, and is called the Rayleigh range
b depth of focus of the beam
M2 beam propagation factor
f1 focal length of the lens
λ laser wavelength
D1 beam diameter at the lens
P laser power
P0 total power transmitted by the beam
Eρ laser energy density
u laser scanning speed
δ laser beam spot size on the powder bed
∆H energy required to melt material
Cp specific heat capacity
∆T temperature difference between ambient and material melting
Lf latent heat of fusion
E melt energy
q heat flux
H amount of the heat flow
r radial distance from point source
T0 environment temperature
α thermal diffusivity
P point source power
u constant moving speed in the same direction of x
x axis of movement
D beam diameter
Q total heat input
η thermal efficiency
ff fraction of the heat deposited in the front quadrant
fr fraction of the heat deposited in the rear quadrant
α contact radius
λe effective contact thermal conductivity
R radius of the sphere
H Hausner ratio
ρT tapped density of powder
ρA apparent density of powder
m mass of sample
Nu Nusselt number
Pr Prandtl number
Re Reynolds number
h heat transfer coefficient
D characteristic length parameter
µ viscosity of the fluid
V velocity of the fluid
Dh hatch distance
List of Acronyms
AM Additive Manufacturing CAD Computer Aided Design
ASTM American Society for Testing and Materials 3D Three-Dimensional
SLM Selective Laser Melting SFF Solid Freeform Fabrication LM Layered Manufacturing SLA Stereolithography UV Ultraviolet
FDM Fused Deposition Modelling ABS Acrylonitrile Butadiene Styrene UC Ultrasonic Consolidation
3D LC Three-Dimensional Laser Cladding LENS Laser Engineered Net Shaping 3DP Three-Dimensional Printing SLS Selective Laser Sintering EBM Electron Beam Melting SLM Selective Laser Melting
DMLF Direct Metal Laser Fabrication
Nd:YAG Neodymium-doped Yttrium Aluminium Garnet TEM Transverse Electromagnetic Mode
LASER Light Amplification Stimulated by Emission of Radiation FCC Face-centred Cubic
BCC Body-centred Cubic UTS Ultimate Tensile Strength SEM Scanning Electron Microscope EBSD Electron backscatter diffraction DSC Differential Scanning Calorimetry DFLUX Defined Heat Flux
FEA Finite Element Analysis FWHM Full Width at Half-maximum
EDX Energy Dispersive X-ray Spectroscopy
In the history of manufacturing, subtractive methods have usually come first, with many machining methods, such as turning, milling, drilling, grinding, etc. In fact, “subtractive manufacturing” is used more as a word to distinguish the traditional mechanical manufacturing methods to the more recent additive manufacturing (AM) method. Although some “additive” fabrication methods like welding and casting have been used in the industry for centuries, they are still considered as traditional manufacturing since they do not employ modern computer aided design (CAD) and manufacturing techniques.
Additive Manufacturing is defined by the ASTM F42 committee in their first standard ASTM F2792-10 as:
“The process of joining materials to make objects from 3D model data, usually layer upon layer, as opposed to subtractive manufacturing technologies.”
During the mechanical manufacturing development history, industry has strived for a more efficient fabrication method with less economic cost. Manufacturing time, raw material and equipment costs, manufacturing sustainability, social and environmental costs have been investigated to develop a revolutionary manufacturing method to benefit both manufacturers and end users.
Additive manufacturing’s early application, Rapid Prototyping, was developed to reduce the fabrication time and cost of developing prototypes of new parts, which was previously achieved by slow and expensive subtractive methods 
manufacturing has moved further to the production end, and is disseminating into the industry and the business world. As a main advantage, additive manufacturing can fabricate very complex geometries which are difficult or impossible to build using conventional manufacturing process . This can bring more profit in some cases for parts made via additive manufacturing than subtractive methods. However, the real integration of additive manufacturing techniques into commercial production is a matter of complementing traditional manufacturing rather than entirely replacing them at the moment .
As one of the AM methods, Selective Laser Melting (SLM) is a process for producing metal parts. It is a laser based additive manufacturing technique, which is able to build complex geometries directly from 3D CAD models, thereby allowing for great design freedom [3-5]. Selective Laser Melting relies on the generation and distribution of laser generated heat to raise the temperature of a region of a powder bed to above its melting point. Due to the high energy input to enable full melting of the powder bed materials, SLM is able to build fully dense metal parts without post heat treatment or infiltration of finished components required .
Successful fabrications of parts by SLM require a comprehensive understanding of the main process controlling parameters such as energy input, powder bed properties and build conditions. The microstructure in SLM parts is a key issue of the process as it strongly affects the final mechanical properties. It is valuable to control the parts’ microstructure through controlling the process parameters to obtain acceptable mechanical properties for end-users. It is important to investigate details of microstructure such as grain size distribution, phase transformation, forming trend on solidification direction, characterisation under different processing parameters, etc. A clear knowledge and reliable prediction of the microstructure forming process will give a better understanding of the SLM process and help other research such as process stability and repeatability study.
In the SLM process, microstructure evolution depends on the thermal history of the process. The temperature distribution in the build area can significantly influence the melting pool behaviour. Due to the high energy input per unit area, non-uniform temperature distribution and fast solidification process, a high thermal gradient may be introduced into the SLM component. This thermal gradient causes residual stresses and affects the final part’s quality 
. Also the presence of a fully molten melt pool makes the process very difficult to control due to increased thermocapillary effects . Therefore, it is important to have an accurate prediction of the temperature distribution history during the process.
1.2 Scope of Research
The aim of this research is to gain a better understanding of the process control parameters in SLM process, and to develop a modelling methodology for the prediction of the foundation of part microstructure. The following objectives were identified to achieve the overall scope of the research.
Investigation of the main laser energy density input control parameters, such as laser power, scanning speed, lens focus position, hatch spacing, etc.
Investigation of the effect of building conditions to the process.
Raw materials characterisation, including powder particle shape and size distribution, flowability, sustainability and their effects to the final parts quality.
Heat transfer model inputs characterisation, such as defining and measuring and the material properties, input loads and boundary conditions.
Establishment of a Finite Element model of moving heat source.
Adding states variable material properties to the heat transfer model.
Establishment of multi-layers heat transfer model.
4 Microstructure prediction based on the knowledge of main process
control parameters and results from heat transfer modelling work.
1.3 Research Methodology
The research is comprised of an experiment and a finite element modelling part.
Experimentation was carried out to understand the effect of each processing control parameters on the final part quality, and to characterise the model inputs. Laser energy input, build conditions and powder bed properties were investigated. Samples were built and tested to gain the knowledge of the relationship between samples’ density and mechanical properties and each process control factor. For laser energy input parameters, laser energy output, scanning strategy and building direction were studied. Build condition investigation includes oxidation control, gas flow in the process chamber and pre-heating study. The powder bed properties study characterises the raw material, which includes chemical composition, particle shape and size distribution, flowability and sustainability examinations. Heat transfer model inputs characterisation, such as defining and measuring the material properties, input loads and boundary conditions were investigated via experiment.
For the predictive modelling of microstructure, a methodology for predicting the temperature distribution history and temperature gradient history during the SLM process has been developed. Moving heat source and states variable material properties were studied and applied to the heat transfer model for reliable prediction. A Multi-layers model was established to simulate the layer by layer process principles. Microstructure was predicted by simulated melting pool behaviour and the history of three dimensional temperature distribution and temperature gradient distribution. These results were validated by relevant experiment examination and measurement.
1.4 Research Novelty
Previous work in the SLM field has focused on the part quality and microstructure control by optimising the laser energy input. This research studies not only the laser energy input, but also raw material properties’ effect on the SLM build quality. Raw material properties are also taken into thermal modelling work for the temperature and microstructure prediction. This research involves a multi-layer heat transfer modelling work to give three dimensional temperature history predictions, while most previous models did not include this layer by layer manner. The results from the model are used for predicting the melt pool behaviour during the SLM process and the microstructure of SLM parts.
1.5 Thesis Structure
Each aspect of this research is described in detail and results are discussed in the remaining chapters of this thesis. A brief description of the contents is given below, with the main structure shown in Figure 1-1.
Chapter 2 Literature Review provides a review of the literature to validate
the relevance of this research. Some of the basic concepts of additive manufacturing process are introduced in the chapter. Previous studies on process control parameters and working principles of SLM are reviewed. Laser manufacturing relevant heat transfer models are studied. The gap of knowledge based on the literature review is identified.
Chapter 3 Experimental Research Methods introduces the research
methods for the experiments in this research. The main equipment is introduced at the beginning, followed by SLM process optimisation, raw material characterisation and model inputs identification methods. Microstructure examination methods are presented at the end.
Chapter 4 Finite Element Modelling Methods introduces the research
methods on simulation establishment. Geometry used in the model, meshing method, boundary condition selection are discussed, as well as the methods on applying the moving heat source, states variable material properties and multi-layers to the model.
Chapter 5 Results & Discussions – SLM Process Control Parameters
studies the effect of laser energy input strategy and building conditions in the SLM process on the final built part quality.
Chapter 6 Results & Discussions – Raw Material Characterisation
characterises the powder’s chemical and physical properties, such as shape, size distribution, flowability, etc. Two samples with different particle size distribution are used in the research. Effects of different particle size distribution on processing parameters optimisation and powder sustainability are investigated.
Chapter 7 Results & Discussions – Model Inputs Characterisation
describes the measurement and calculation of the main heat transfer model inputs, which including input heat source, base material properties and boundary conditions.
Chapter 8 Results & Discussions – Heat Transfer Model Establishment
provides the main work on the heat transfer model establishment – the procedure of applying moving heat source, states variable material properties and boundary conditions into the simulation. This chapter also presents the multi-layers model establishment procedure and discusses the results from simulation.
Chapter 9 Results & Discussions – Microstructure Prediction and Validation focuses on the microstructure prediction using the results
obtained from previous chapter, and the validation through experiment examinations.
Chapter 10 Discussions discusses the experimental and the modelling
results presented in previous chapters and their connections.
Chapter 11 Conclusions and Future Work presents the main conclusions
from the research, along with the suggested future work.
2 Literature Review
2.1 Additive Manufacturing
Additive Manufacturing (AM) is a group of manufacturing technologies which are capable of producing 3D solid parts by adding successive layers of material. Parts are fabricated in an additive manner, layer by layer; and the geometric data can be taken from a CAD model directly [3, 4, and 9]. The main revolutionary aspect of AM is the ability of quickly producing complex geometries without the need of tooling, allowing for greater design freedom . The other advantages include the reduction in manufacturing steps and use of materials; therefore causing reduction in fabricating cost. Additive Manufacturing is also referred to as Solid Freeform Fabrication (SFF) , Layered Manufacturing (LM) , and e-Manufacturing .
Additive Manufacturing can go back to the late 1980’s, early 1990’s [13, 14] . In 1991, CIRP’s STC-E devoted a first keynote paper on a survey of additive manufacturing, which surveys one decade of innovation in AM . Although most processes were already known in 1991, most of them were still in a pre-commercial stage, with some of them reaching the commercialisation stage painfully . The first successful process, Stereolithography from 3D systems, came out in 1991. Followed by other companies, there is a clear breakthrough in 1994 in AM at which time machine sales took off exponentially . Many AM techniques existing today can process materials such as polymers, metals, ceramics and composites. The bonding of material can be achieved by different physical and chemical methods.
The classification of AM technologies can be based on the raw material used in the process , which divides these technologies into three different categories: Liquid-based processes, Powder-based processes and Solid-based processes. Figure 2-1 shows a family tree of AM technologies. It may not cover all current technologies, but it shows the categorisation of major AM techniques.
Figure 2-1 Family tree of Additive Manufacturing Technologies 
TechnologiesLiquid-based Stereolithography Jetting Systems Direct Light Processing
Hign-Viscosity Jetting The Maple Process
Selective Laser Sintering Directing Metal Laser
Sintering Three-Dimensional Printing
Fused Metal Deposition Electron Beam Melting Selective Laser Melting Selective Masking Sintering Selective Inhibition Sintering Electrophotographic Layered
Manufacturing High-Speed Sintering
Fused Depostion Modelling Laminated Object
Manufacturing Ultrasonic Consolidation
2.1.2 Liquid-based processes
Most Liquid-based AM systems form solid parts by selectively curing regions of photosensitive polymers using a particular wavelength of light. The light source can be either a scanning laser beam or a wide area light source. Photocurable resins which can achieve stable properties over time and in different environments are widely used in Liquid-based additive manufacturing technologies .
Stereolithography (SLA) system, released by 3D systems in 1987, is widely
considered to be the founding process within the field of AM . The stereolithography process uses an ultraviolet (UV) laser to cure a photocurable resin. Parts can be built from a CAD model and the whole process can be controlled by the machine’s software, including automatically generating the supports.
2.1.3 Solid-based processes
AM processes which use solid raw materials in non-powder form have been an integral part of the AM industry since early 1990s . They are still developed and improved by both the suppliers and academic institutions today.
Fused Deposition Modelling (FDM) was commercialised by Stratasys Inc.
in 1991 [8, 18]. In this process, solid wire-shaped materials are heated to a semi-molten consistency before depositing using single or multi nozzle systems. The nozzle systems traverse in X and Y direction to create a two-dimensional layer. FDM can process materials such as polycarbonate, polyphenylsulfone and acrylonitrile butadiene styrene (ABS). This process can build solid parts with little waste, but the size of the extrusion limits the size that any features smaller than double the track width cannot be produced .
Ultrasonic Consolidation (UC) is also a solid-based technology developed
by Solidica Inc. in 2002 . It combines the ultrasonic welding of metal foils and additive manufacturing techniques to produce solid parts. The process applies sonic oscillations to metal foil under an applied load. The oscillation bonds the thin metal foil together with a very low heat. This process is capable to process a range of metals such as Iron, Copper, Nickel and dissimilar combinations like Al/Stainless steel and Al/Ni .
2.1.4 Powder-based processes
Powder-based additive manufacturing technologies offer a wide range of material possibilities such as polymers, metals and ceramics. Parts can be built with similar material properties and stability compared with solid material. These technologies can be divided into two main types: powder feed deposition and powder bed deposition.
Based on powder feed deposition, a number of processes have been developed, such as Three-Dimensional Laser Cladding (3D LC) which is also called Laser Engineered Net Shaping (LENS) . In the process, the powder is delivered in a gas jet through nozzles, coaxially with the laser beam. The powder in the melt pool created by the laser can form a cladding line and then cool to form a solid structure when the laser moves away. It is important to melt the powders and homogenise the melt pool for successful building . Fully dense parts can be achieved by this technique [22-24].
Three-Dimensional Printing (3DP) developed at MIT is the basis of a
number of technologies that use the application of a binder to a powder layer to construct parts [16-18, 25]. In the process, a thin powder layer is selectively bonded by ink-jet droplets of adhesive binder. A range of materials can be used in this technique, including metals. But the parts fabricated by this technique usually have high surface roughness and need further post processing operations to obtain final properties [26, 27].
Selective Laser Sintering (SLS) is an important additive manufacturing
technique widely used today, which is referred to as powder bed deposition. It was first invented in 1979 by Ross Householder, and commercialised in the late 1980s by the University of Texas at Austin, when the first machine came out in 1992 developed by DTM Corporation [28-30]. The process is in many ways similar to Stereolithography; but is capable of processing a variety of materials including polymers, metals and ceramics. The powdered raw material is sintered or partially melted by a laser which selectively scans the surface of the powder bed to create a two-dimensional solid shape, and then a fresh layer of powder is added to the top of the bed to form another solid layer which can be traced by the laser bonding it to the layer below. It is basically a one-step process and you can get the final parts directly from a CAD model. To minimise the required laser output energy and to reduce thermal stresses, the powder is normally maintained at an elevated temperature, just below its fusing point [28-32]. To avoid oxidation problem during the process, it usually operates in an inert protect gas environment .
Electron Beam Melting (EBM) is a process very similar to SLS but replaces
the laser with an electron beam. It was developed by Arcam in Gothenburg Sweden in 1997 .The electron beam is stationary and there is no need for scanning mirrors as the beam can be directed by changing an electromagnetic field, which allows for high scanning speed and fast build rates . The technique offers the ability to fully melt a wide range of metal powders due to the high power developed by the electron beam. However the process is limited to conductive materials and surfaces .
Selective Laser Melting (SLM) is also a process very similar to SLS, but it
uses a higher energy density to enable full melting of the powder. This technique is capable of building fine details such as thin vertical walls, complex lattice structures and fine cylindrical struts [35, 36]. SLM is capable of processing many standard metal materials like Stainless Steel, Inconel, Titanium alloys and Aluminium alloys [16, 25]. Due to the high temperature involved in processing metals, the use of a protecting gas is important to avoid oxidation. It can also enhance the wet-ability of the molten material and
reduce the porosity caused by oxidation . However, due to full melting process and high temperature, there can be big thermal stresses and large shrinkage after solidification, which need to be improved.
2.2 Direct Metal Laser Fabrication
Direct Metal Laser Fabrication (DMLF) is a group of laser based additive manufacturing technologies for producing metal components. The laser beam is delivered to the surface of the material, and the heat generated by the laser causes the material to sinter or completely melt. When the laser beam moves away, the material can be cooled and forms solid parts. The material type can be in powder or wire form, and the laser types and material deposition methodology can vary . Due to the accuracy, stability and versatility of the laser beam, DMLF processes are capable of building end-use parts with acceptable accuracy and resolution just in one step. Also, these technologies can fabricate parts with improved mechanical properties compared to the conventionally processed, such as casting and forging [38, 39].
2.2.1 Laser scanning systems
DMLF processes can vary due to system configuration. The type of laser used within the system is a significant factor that greatly affects the capabilities of the system. With the continuous development of laser technology, many kinds of lasers have been used in laser direct manufacturing. Commercial sintering and melting machines have used Carbon Dioxide (CO2), Neodymium-doped Yttrium Aluminium Garnet (Nd:YAG) and Ytterbium (Yb) fibre lasers. The main difference between these lasers is their wavelength. CO2 lasers have a wavelength of 10.6µm while Nd:YAG and Yb fibre lasers have wavelengths in the range of 1.06 to 1.1µm.
As a gas laser, CO2 lasers are one of the highest-power continuous wave lasers that are currently available. It is also quite efficient: the ratio of output power to pump power can be as large as 20% . Nd:YAG lasers are solid-state lasers, which can operate in both pulsed and continuous mode. Pulsed Nd:YAG lasers are typically operated in the so called Q-switching mode, which can generate high intensity . Yb fibre lasers are capable of producing several-kilowatt of continuous power, having 70-80% optical-to-optical and up to 25% electrical-to-optical-to-optical efficiency . The advantage of the fibre laser is that the light can be coupled into the flexible fibre and can be delivered to a movable focusing element with high output power and high optical quality .
The Gaussian distribution is the most widely adopted model for laser intensity distribution, which utilises the symmetrical distribution to describe laser intensity across the laser beam . It assumes that in most cases the maximum laser intensity is at the centre of the beam. Figure 2-2 shows three different Transverse Electromagnetic Mode (TEM) radial intensity distributions. The TEM00 profile is the one suited for laser machining due to high energy concentration in the central area and also the energy is gradually emitted from the centre, which delivers enough and smooth energy to the substrate .
Based on the Gaussian function, the corresponding time-averaged intensity distribution can be given by Equation (2.1) .
( ) | ( )| ( ( )) (
( )) (2.1) where r is the radial distance from the centre axis of the beam, z is the axial distance from the beam's narrowest point (the "waist"), ( ) is the intensity at the centre of the beam at its waist, w(z) is the radius at which the field amplitude and intensity drop to 1/e and 1/e2 of their axial values respectively, and w0 = w(0) is the waist size. The constant is the characteristic impedance of the medium in which the beam is propagating, and for free space, .
For a Gaussian beam of wavelength λ at a distance z along the beam from the beam waist, the variation of the spot size w(z), can be given by Equation (2.2).
( ) √ ( ) (2.2)
Where zR is the distance along the propagation direction of the laser beam from the waist to the place where the area of the cross section is doubled, and is called the Rayleigh range , given by Equation (2.3). The distance b between two Rayleigh range points is the depth of focus of the beam, where b=2zR.
The waist size, which is the minimum spot diameter to a Gaussian beam, can be given by Equation (2.4) .
Where M2 is the beam propagation factor, f1 is the focal length of the lens, λ is the laser wavelength and D1 is the beam diameter at the lens. Figure 2-3 shows these beam parameters stated above.
Figure 2-3 Gaussian beam parameters after focusing 
The power P passing through a circle of radius r in the transverse plane at position z can be given by Equation (2.5) .
( ) [ ( )] (2.5)
where P0 is the total power transmitted by the beam, given by Equation (2.6) 
Similarly combining these two functions can find that about 95% of the beam’s power will flow through a circle of radius r=1.224w(z) 
The peak intensity at an axial distance can be calculated using L'Hôpital's rule, given by Equation (2.7), which is twice the average intensity .
[ ( )]
( ) (2.7) A whole laser scanning system usually has several optical components. A beam expander is often used where the beam path is long or the laser produces such a small beam diameter which is very difficult to focus without
having the focal lens close to the work piece. Different types of reflecting mirrors are used to direct the laser beam in the X and Y axis. A focal lens is used to focus the laser beam where the minimum spot size can be on the surface of the building platform.
2.2.2 Laser-Material interactions
Laser light is a form of energy or electromagnetic radiation generated by Light Amplification Stimulated by Emission of Radiation (LASER). It can also be considered as moving particles with very high energy values. The process of melting using a laser begins by converting the laser’s photons into kinetic energy . The photons can excite electrons which are in the outmost shell of surface atoms of the target material, including the release and excitation of conduction electrons. This energy transfer usually takes a very short time, about 1ps in metals ; so it is revealed as rapid heating or thermalisation. The heat generated by the laser will travel through the target material by thermal conduction, and can completely liquefy the material to form a melt pool.
When the laser transfers energy to a material, the energy cannot be fully absorbed by the material. The absorption of a material is defined as the ratio of the absorbed radiation to the incident radiation . The value of the absorption coefficient will vary with the same effects that affect the reflectivity. For most materials,
Reflectivity = 1 – absorptivity – transmission 
In actual processes, the energy loss contains radiation, convection with the surrounding atmosphere and expulsion of materials . However, the main loss of the laser energy is reflection .
In general, the absorption depends on the laser wavelength, the nature of the material, surface geometry, surrounding gas and temperature, etc. [56-59] It is
believed that at longer wavelengths metallic materials generally have an increased reflectivity and consequently the laser processing of metals is more difficult, so it is preferable to process metals using lasers with shorter wavelengths as the metal can absorb more energy from the laser . This is because of resonance and scattering effects of the laser wavelength .
Unlike an opaque continuous medium, the powder bed allows a certain penetration of the light energy of the laser beam through gaps between particles and mutiple reflection into particles. This penetration allows more laser energy absorption into the powder bed rather than a continuous medium. In order to describe how the energy will be absorbed in depth, an "energy penetration" parameter was introduced . Table 2-1 shows the absorption of some typical powder materials at different wavelengths.
Material λ= 1.06µm λ= 10.6µm Cu 59% 26% Fe 64% 45% Sn 66% 23% Ti 77% 59% Ni-alloy 64% 42% NaNO3 16% 80% NaCl 17% 60%
Table 2-1 Absorption of powder materials at different wavelength 
2.2.3 Binding mechanisms
There are many ways to consolidate metal powder material pre-deposited on a building platform with a laser. Classification of laser based powder
consolidation mechanisms can be based on the powder material state, which divides these ways into three different categories: Solid State Sintering, Liquid Phase Sintering/Partial Melting and Full Melting .
Solid State Sintering is a consolidation process occurring below the material’s melting temperature. This binding creates “necks” between powder particles without the presence of a liquid phase at the contact areas [64, 65]. This method is rarely used in additive manufacturing as diffusion of atoms is very slow and not compatible with the desired high laser scanning speed which will increase the process productivity and economic feasibility .
Liquid Phase Sintering and Partial Melting include many binding mechanisms in which part of the powder material with low melting temperature is melted while the remaining material with a higher melting temperature remains solid. There is a limited degree of rearrangement of the solid particles due to the short interaction time; so that the metal part produced directly using partial melting will contain a high level of porosity . It may need post-processing operations in order to reduce the part porosity and improve mechanical properties.
Full melting is a consolidation mechanism which is capable of producing fully dense parts without the need of any post-processing. It can achieve this by completely melting the powder particles with the use of high laser energy densities. However, due to the high temperature gradients and densification ratio during the process, high internal thermal stresses can be generated [66, 67]
. Also, balling and dross formation from the melt powder materials in the melt pool may result in poor surface finish . Explanation on the balling effect can be found in section 2.3.3.
2.3 Selective Laser Melting
Selective Laser Melting (SLM) is a powder bed process which is very similar to Selective Laser Sintering (SLS), but uses a different laser energy density
to enable full melting of the powder; a schematic of the process is shown in Figure 2-4. Theoretically the fabricated parts can exhibit full or near-full density without any post processing work such as heat treatment or infiltration of finished components required .
SLM can process standard metal powder materials like stainless steel, Inconel, titanium alloys and aluminium alloys. These powders are processed directly without the addition of a binder. The ability to fabricate parts using single type of metal powder material is one of the biggest advantages of SLM 
. Recently, it has been found that SLM can also build from mixture powder 
Figure 2-4 Schematic of the Selective Laser Melting process
2.3.1 Process control factors
The SLM control factors which influence part physical and mechanical properties include laser energy input strategy, raw material properties, powder bed properties, building strategy and atmosphere . Previous
studies performed using SLM have shown that important part features such as porosity, surface roughness, geometry, parts dimensional accuracy and microstructure are strongly dependent on the system’s laser processing parameters such as laser power, scanning speed, layer thickness, scan overlap, etc. [70-72]
Some factors in the process are controllable, while some not. Table 2-2 shows the main SLM control parameters classified by controllability and also different control parts in the process.
Control Systems Variable Parameters Non-variable Parameters
Optical scanning system
Laser power Laser focus position Beam energy intensity
Laser efficiency Laser beam profile Focal lens properties
Process scanning strategy Scanning speed Hatch distance Layer thickness Scanning direction Re-melting scan Processing environment Gas flow Pre-heating Building substrate thickness Inert gas
Raw material & powder bed
Particle shape Particle size distribution
Powder flowability Density of the powder
Chemical compositions Laser energy absorption
2.3.2 Optical scanning system
Optical scanning systems used in SLM today for processing metals usually contains a short pulse or continuous wave of laser energy, a beam expander, a dual axis scanning mirror system and a F-Theta focal length lens. The use of F-theta lens can provide a flat field at the image plane of scan, delivering the laser energy uniformly throughout the powder bed, shown in Figure 2-5. The development of F-Theta lens covers a wider spectral range of laser and provides a larger working area, which increases the efficiency of laser material processing techniques .
Figure 2-5 Working principle of F-theta lens 
The main feature of a continuous wave laser is it has a continuous laser output due to the continuous excitation of the reactive medium where the energy output is theoretically constant. In this case, the powder bed can receive a continuous stable energy input and be heated and melt continuously . However, in some SLM processes, laser energy is emitted in a pulse mode by setting the exposure time and the distance between exposures. This method of laser energy delivery is carried out such that heat build-up and melt pool width is minimised .
In SLM processes, laser energy density, Eρ, is a key factor that affects the final part’s quality. Laser energy density is defined by the incident laser power P (W), laser scanning speed u (mm/s) and laser beam spot size on the powder bed δ (mm), given by Equation (2.9) 
( ) (2.9) The process parameters, laser power and scanning speed can be controlled during the process through machine control software. Laser beam spot size on the powder bed can also be controlled by adjusting the lens position or the distance between lenses in the beam expander. In some systems, beam offset is used to compensate for the laser beam focal diameter at the boundaries of the scanned section .
2.3.3 Process scanning strategy
In SLM processes, the input process parameters can be controlled and varied to achieve the resultant parts. Many previous input parameter control works have been carried out to improve the material properties such as density, surface finish, accuracy and mechanical properties. These machine controllable input parameters include laser exposure time and point distance, powder layer thickness, hatch type, hatch distance, beam offset, and other strategies. Table 2-3 and Figure 2-6 show the description of some brief parameters.
Figure 2-6 Schematic of some input process parameters Each circle presents
one laser exposure point
laser moving direction
Input Parameters Description
Exposure time Determines the time of laser exposure into each point.
Point distance Each hatch line is divided into a series of points, point centres are separated by the point distance.
Scanning speed Defines the speed of the scanning laser movement.
Layer thickness Specifies the layer incremental distance during process.
Hatch type Controls the scanning strategy, such as scanning direction, re-melting scan, chessboard scan, etc.
Hatch distance Controls the distance between two adjacent lines of the scan.
Table 2-3 Input process parameters of SLM
A characteristic of the SLM process is the combination of exposure time and point distance, which is used to define the scanning speed of the laser beam:
( ) ( ) (2.10)
Scanning speed is a main factor than can affect the laser energy density. It must be mentioned that a range of laser powers and scanning speeds can produce the same energy density. However, the effect on the powder can be variable as some significant effect factors such as radiation and absorption can be different . Hatch distance also affects the laser energy density.
The main aim of controlling the energy density is to make sure the heat absorbed by the powder is enough for producing dense parts without
heating. High energy density can cause the surface powder to begin to vaporise before a significant depth of molten material is achieved. It can also cause deformation of the parts due to high thermal stresses. Reducing the energy density can be achieved by reducing the laser power, increasing the scanning speed and increasing the hatch distance. The melt powder layer thickness decreases with increasing the scanning speed due to the shorter interaction time, this thickness also decreases with increasing hatch distance [4, 76]
Controlling the process parameters needs to consider the wet-ability for avoiding balling phenomenon. Balling is when melting is induced by the laser beam, the molten powder quickly consolidates into spheres of diameter approximately equal to the diameter of the laser beam, rather than consolidating into the previous layer. Previous work showed that the spherical structure increased with decreasing the scanning speed and increasing the laser power [77-79]. Recent investigation indicated that the scanning speed is the main factor in determining / avoiding the balling phenomenon . Suitable higher scanning speed can reduce balling, even when the energy densities are the same.
Many scanning strategies can affect the melt pool behaviour and material properties of the parts . A widely used melting strategy is used to re-melt the surface of the part to reduce the top surface roughness . It needs a control of the process parameters like scanning speed and input power to ensure the efficient re-melting results.
2.3.4 Process environment
In the SLM process, the gas chamber should be filled with a protecting gas to aid reduced oxidation during the process. Oxygen can react with the molten material causing the surface to oxidise which will affect the final part properties. Oxidation can cause the reduction of molten material wet-ability, which can be a barrier to successful layer fusion and can cause porosity,